#------------------------------------------------------------------------------
#$Date: 2016-02-20 05:06:23 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176774 $
#$URL: svn://www.crystallography.net/cod/cif/2/20/44/2204465.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2204465
loop_
_publ_author_name
'Li, Zong-Xiao'
'Zhang, Xin-Li'
_publ_section_title
;
 Tetrapyridinedithiocyanatocopper(II)
;
_journal_issue                   11
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              m1597
_journal_page_last               m1598
_journal_paper_doi               10.1107/S160053680402495X
_journal_volume                  60
_journal_year                    2004
_chemical_formula_iupac          '[Cu(N C S)2 (C5 H5 N)4]'
_chemical_formula_moiety         'C22 H20 Cu N6 S2'
_chemical_formula_sum            'C22 H20 Cu N6 S2'
_chemical_formula_weight         496.10
_chemical_name_systematic
;
Tetrapyridinedithiocyanatocopper(II)
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.245(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   12.420(2)
_cell_length_b                   12.999(2)
_cell_length_c                   15.180(3)
_cell_measurement_reflns_used    3236
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      27.310
_cell_measurement_theta_min      2.324
_cell_volume                     2340.6(7)
_computing_cell_refinement       SMART
_computing_data_collection       'SMART (Bruker, 1998)'
_computing_data_reduction        'SAINT (Bruker, 1998)'
_computing_molecular_graphics    SHELXTL
_computing_publication_material  SHELXTL
_computing_structure_refinement  SHELXTL
_computing_structure_solution    'SHELXTL (Bruker, 1998)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker SMART CCD area-detector'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0235
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            6801
_diffrn_reflns_theta_full        26.50
_diffrn_reflns_theta_max         26.50
_diffrn_reflns_theta_min         2.32
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.132
_exptl_absorpt_correction_T_max  0.8221
_exptl_absorpt_correction_T_min  0.7572
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 1996)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.408
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Block
_exptl_crystal_F_000             1020
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.18
_refine_diff_density_max         0.538
_refine_diff_density_min         -0.473
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     142
_refine_ls_number_reflns         2425
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.071
_refine_ls_R_factor_all          0.0497
_refine_ls_R_factor_gt           0.0449
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0816P)²+3.7197P] where P = (Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1415
_refine_ls_wR_factor_ref         0.1456
_reflns_number_gt                2117
_reflns_number_total             2425
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            ci6461.cif
_cod_data_source_block           I
_cod_original_cell_volume        2340.7(7)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               2204465
_cod_database_fobs_code          2204465
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Cu1 0.2500 0.2500 0.5000 0.0435(2) Uani d S 1 Cu
S1 0.57369(8) 0.14417(8) 0.41851(7) 0.0641(3) Uani d . 1 S
N1 0.1376(2) 0.12066(19) 0.43985(17) 0.0442(6) Uani d . 1 N
N2 0.2875(2) 0.18854(19) 0.64226(16) 0.0429(5) Uani d . 1 N
N3 0.3873(2) 0.1712(2) 0.48165(18) 0.0477(6) Uani d . 1 N
C1 0.1709(3) 0.0231(3) 0.4526(3) 0.0570(8) Uani d . 1 C
H1 0.2458 0.0099 0.4849 0.068 Uiso calc R 1 H
C2 0.1007(4) -0.0596(3) 0.4208(3) 0.0713(11) Uani d . 1 C
H2 0.1275 -0.1265 0.4329 0.086 Uiso calc R 1 H
C3 -0.0079(4) -0.0418(3) 0.3716(3) 0.0774(12) Uani d . 1 C
H3 -0.0570 -0.0962 0.3492 0.093 Uiso calc R 1 H
C4 -0.0439(3) 0.0579(4) 0.3556(3) 0.0760(12) Uani d . 1 C
H4 -0.1178 0.0722 0.3212 0.091 Uiso calc R 1 H
C5 0.0302(3) 0.1367(3) 0.3910(2) 0.0569(8) Uani d . 1 C
H5 0.0044 0.2041 0.3804 0.068 Uiso calc R 1 H
C6 0.3420(3) 0.0998(3) 0.6668(2) 0.0533(8) Uani d . 1 C
H6 0.3669 0.0652 0.6229 0.064 Uiso calc R 1 H
C7 0.3639(3) 0.0561(3) 0.7532(3) 0.0656(10) Uani d . 1 C
H7 0.4013 -0.0065 0.7666 0.079 Uiso calc R 1 H
C8 0.3290(3) 0.1074(4) 0.8187(3) 0.0716(11) Uani d . 1 C
H8 0.3426 0.0804 0.8777 0.086 Uiso calc R 1 H
C9 0.2742(4) 0.1988(4) 0.7957(3) 0.0719(11) Uani d . 1 C
H9 0.2500 0.2350 0.8392 0.086 Uiso calc R 1 H
C10 0.2546(3) 0.2376(3) 0.7071(2) 0.0548(8) Uani d . 1 C
H10 0.2172 0.3001 0.6924 0.066 Uiso calc R 1 H
C11 0.4650(2) 0.1593(2) 0.45602(19) 0.0402(6) Uani d . 1 C
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
N3 Cu1 N3 7_556 . 180.00(14) yes
N3 Cu1 N1 7_556 . 89.25(10) yes
N3 Cu1 N1 . . 90.75(10) yes
N3 Cu1 N1 7_556 7_556 90.75(10) ?
N3 Cu1 N1 . 7_556 89.25(10) ?
N1 Cu1 N1 . 7_556 180.00(8) yes
N3 Cu1 N2 7_556 7_556 90.54(10) ?
N3 Cu1 N2 . 7_556 89.46(10) yes
N1 Cu1 N2 . 7_556 86.97(9) yes
N1 Cu1 N2 7_556 7_556 93.03(9) ?
N3 Cu1 N2 7_556 . 89.46(10) ?
N3 Cu1 N2 . . 90.54(10) yes
N1 Cu1 N2 . . 93.03(9) yes
N1 Cu1 N2 7_556 . 86.97(9) ?
N2 Cu1 N2 7_556 . 180.0 yes
C1 N1 C5 . . 116.5(3) ?
C1 N1 Cu1 . . 122.4(2) ?
C5 N1 Cu1 . . 121.1(2) ?
C6 N2 C10 . . 116.7(3) ?
C6 N2 Cu1 . . 121.7(2) ?
C10 N2 Cu1 . . 121.6(2) ?
C11 N3 Cu1 . . 156.0(2) ?
N1 C1 C2 . . 123.7(4) ?
N1 C1 H1 . . 118.1 ?
C2 C1 H1 . . 118.1 ?
C3 C2 C1 . . 119.0(4) ?
C3 C2 H2 . . 120.5 ?
C1 C2 H2 . . 120.5 ?
C2 C3 C4 . . 118.6(4) ?
C2 C3 H3 . . 120.7 ?
C4 C3 H3 . . 120.7 ?
C3 C4 C5 . . 119.3(4) ?
C3 C4 H4 . . 120.3 ?
C5 C4 H4 . . 120.3 ?
N1 C5 C4 . . 122.9(4) ?
N1 C5 H5 . . 118.6 ?
C4 C5 H5 . . 118.6 ?
N2 C6 C7 . . 124.1(3) ?
N2 C6 H6 . . 117.9 ?
C7 C6 H6 . . 117.9 ?
C8 C7 C6 . . 118.3(4) ?
C8 C7 H7 . . 120.8 ?
C6 C7 H7 . . 120.8 ?
C9 C8 C7 . . 118.7(3) ?
C9 C8 H8 . . 120.6 ?
C7 C8 H8 . . 120.6 ?
C8 C9 C10 . . 119.7(4) ?
C8 C9 H9 . . 120.2 ?
C10 C9 H9 . . 120.2 ?
N2 C10 C9 . . 122.5(4) ?
N2 C10 H10 . . 118.8 ?
C9 C10 H10 . . 118.8 ?
N3 C11 S1 . . 179.0(3) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Cu1 N3 7_556 2.077(2) ?
Cu1 N3 . 2.077(2) yes
Cu1 N1 . 2.203(2) yes
Cu1 N1 7_556 2.203(2) ?
Cu1 N2 7_556 2.219(2) ?
Cu1 N2 . 2.219(2) yes
S1 C11 . 1.625(3) ?
N1 C1 . 1.330(4) ?
N1 C5 . 1.336(4) ?
N2 C6 . 1.334(4) ?
N2 C10 . 1.334(4) ?
N3 C11 . 1.154(4) ?
C1 C2 . 1.378(5) ?
C1 H1 . 0.93 ?
C2 C3 . 1.353(7) ?
C2 H2 . 0.93 ?
C3 C4 . 1.370(6) ?
C3 H3 . 0.93 ?
C4 C5 . 1.375(5) ?
C4 H4 . 0.93 ?
C5 H5 . 0.93 ?
C6 C7 . 1.380(5) ?
C6 H6 . 0.93 ?
C7 C8 . 1.370(6) ?
C7 H7 . 0.93 ?
C8 C9 . 1.361(7) ?
C8 H8 . 0.93 ?
C9 C10 . 1.389(5) ?
C9 H9 . 0.93 ?
C10 H10 . 0.93 ?
